Producing Bulk Ultrafine-Grained Materials by Severe Plastic Deformation: Ten Years Later
- 3.5k Downloads
It is now well established that the processing of bulk solids through the application of severe plastic deformation (SPD) leads to exceptional grain refinement to the submicrometer or nanometer level. Extensive research over the last decade has demonstrated that SPD processing also produces unusual phase transformations and leads to the introduction of a range of nanostructural features, including nonequilibrium grain boundaries, deformation twins, dislocation substructures, vacancy agglomerates, and solute segregation and clustering. These many structural changes provide new opportunities for fine tuning the characteristics of SPD metals to attain major improvements in their physical, mechanical, chemical, and functional properties. This review provides a summary of some of these recent developments. Special emphasis is placed on the use of SPD processing in achieving increased electrical conductivity, superconductivity, and thermoelectricity, an improved hydrogen storage capability, materials for use in biomedical applications, and the fabrication of high-strength metal-matrix nanocomposites.
KeywordsSevere Plastic Deformation Severe Plastic Deformation Processing Severe Plastic Deformation Technique Nanostructural Feature Vacancy Agglomerate
Processing through the application of severe plastic deformation (SPD) has now become widely accepted as a promising tool for the fabrication of bulk ultrafine-grained (UFG) materials. An earlier report defined the terms associated with this type of processing1 and the various experimental procedures that may be used to achieve grain refinement to the submicrometer or even the nanometer level. The present article, published 10 years later, describes the more recent developments in this rapidly expanding research field with special emphasis on the potential for achieving exceptional physical, mechanical, and functional properties that cannot be attained through the use of conventional techniques. New activities, including a classic development within the general framework of SPD processing, have been described in several recent reviews,2, 3, 4, 5, 6, 7, 8, 9, 10, 11, 12, 13, 14 but the present article offers the first opportunity to provide a more detailed overview of some of the important developments since the earlier article in 2006.
New Properties Achieved Through SPD Processing
The effect of processing by SPD is not limited to extreme grain refinement. Indeed, processing by SPD may also result in unusual phase transformations associated with the dissolution of second phases, precipitation, amorphization, and other processes that produce various nanostructural features. These include deformation twins, nonequilibrium grain boundaries, dislocation substructures, vacancy agglomerates, solute segregation, and clusters.7,9,12 These changes in the inner makeup of the material may affect the deformation mechanisms and, consequently, change a material property in a radical way. As a result, new structural and functional metals and alloys with uniquely superior properties can be developed by SPD processing.8,9,13 The following sections present several recent examples of extraordinary properties achieved by SPD processing that convincingly demonstrate the large innovation potential of bulk nanomaterials.
Currently, many different SPD processing techniques are available,3,9,10,12 but most attention to date has concentrated on two processes: equal-channel angular pressing (ECAP) and high-pressure torsion (HPT). Both are especially attractive for research because they produce materials having smaller grain sizes and higher fractions of high-angle grain boundaries than most other SPD techniques.3,5 These two main techniques are applied in the examples now described.
Strength and Ductility of UFG Materials Processed by SPD
It has been a perpetual endeavor for materials scientists to make materials with both high strength and high ductility.15,16 This issue has become more urgent under the current challenge of global warming and the energy crisis. Stronger materials can make transportation vehicles lighter and consequently more energy efficient. UFG materials processed by SPD techniques usually have much higher strength than their coarse-grained (CG) counterparts.13 However, improving their poor ductility without sacrificing their strength has been challenging. This problem is further compounded by the confusion of ductility with plasticity in the academic community and the difficulty of using standard samples to measure the ductility of UFG materials.
Ductility is measured under tensile loading, and can be considered a special case of plasticity, i.e., tensile plasticity. At room temperature, ductility is controlled largely by the strain-hardening capability and, to a lesser extent, the strain rate sensitivity of the flow stress. At higher temperatures, the strain rate sensitivity is high, which may considerably improve the ductility. Ductility is significantly affected by the microstructure, such as grain size, and the distribution of second-phase particles. On the other hand, plasticity is largely determined by the intrinsic properties of a metal such as the crystal structure and, in particular, the availability of the slip systems and dislocation mobility. For example, hexagonal-close-packed (hcp) metals commonly have lower plasticity than face-centered-cubic (fcc) and body-centered-cubic (bcc) metals.
To improve the ductility of UFG metals, the most effective way is to increase their strain-hardening rate. In other words, it is necessary to design UFG structures that can effectively block and accumulate dislocations. Grain boundaries are no longer effective for dislocation accumulation because, when the grain sizes are very small, grain boundaries become dislocation sources and sinks without much dislocation accumulation.17 It follows that dislocation barriers are required within the grain interior where dislocations can be blocked and accumulate. Some successful strategies to this end include the use of growth twins,18 deformation twinning,19, 20, 21 stacking faults,22,23 and second-phase particles/precipitates24 as barriers. Since these approaches can also increase the strength, they often lead to a simultaneous increase in both strength and ductility. It should also be noted that UFG metals processed by SPD techniques often contain a high density of dislocations. This leaves little room for dislocation accumulation during tensile testing before saturation is reached. Therefore, annealing to lower the dislocation density without increasing the grain size is expected to improve the strain hardening and ductility. Indeed, it has been found that processing the UFG metals to a very large strain or annealing SPD-processed UFG metals for a very short time can enhance the ductility,20,25,26 which could be due to both a lower dislocation density and a higher fraction of high-angle grain boundaries.
It should be noted that for UFG metals and alloys with low melting temperatures, room temperature may represent a relatively high homologous temperature that, coupled with the small grain size, may lead to grain boundary sliding during deformation and consequently to high strain rate sensitivity to enhance ductility.27, 28, 29
Fabricating High-Strength Metal-Matrix Nanocomposites by High-Pressure Torsion
Processing by HPT is usually undertaken on disk-shaped specimens,31 although the processing has been extended also to cylindrical32, 33, 34 and sheet35 samples. The conventional HPT disks are generally cut from a single metal or alloy, but recently it was shown that semicircular disks of Al and Cu may be successfully bonded through a solid-state reaction at ambient temperature by using HPT processing through up to 100 turns.36 A similar procedure was used later in which separate disks of commercial-purity aluminum and a commercial ZK60 magnesium alloy, cut and polished to thicknesses of ~0.8 mm, were stacked in the HPT facility as three disks in the sequence Al/Mg/Al and processed by HPT at room temperature under an applied pressure of 6.0 GPa.37 This processing was conducted under quasi-constrained conditions in which there is a small outflow of material around the periphery of the stack during the processing operation.38
Inspection of the stacked disks after processing revealed Al-rich and Mg-rich phases, but near the edges of the disks after five and ten turns there was a homogeneous distribution of very fine Mg phases confined within the Al matrix. Furthermore, careful microstructural analysis revealed a true nanostructure in the Al-Mg disks after processing with average grain sizes near the edges of the disks of ~190 nm and ~90 nm when processing through five and ten turns, respectively.37 It was shown by using energy-dispersive x-ray spectroscopy (EDS) that an intermetallic compound, β-Al3Mg, was formed in the Al matrix as thin layers with thicknesses of ~20 nm and ~30 nm after five and ten turns, respectively, thereby producing an intermetallic-based, Al metal-matrix nanocomposite in the highly deformed regions near the edges of the disks. In addition, an intermetallic compound of γ-Al12Mg17 was identified in the Al matrix using x-ray diffraction, and this was attributed to rapid diffusion of Mg from the Mg-rich phases.37 Measurements of the Vickers microhardness, Hv, revealed a very significant increase in hardness to Hv = 135 near the edge of the disk after five turns and an even higher hardness of Hv = 270 near the edge after ten turns. This hardness was attributed to a combination of Hall–Petch strengthening, solid solution strengthening, and precipitation hardening where these strengthening processes can occur simultaneously because of the use of very rapid processing at a relatively low temperature that prevents the occurrence of significant recovery. It is important to note that the hardness values in the pressed material are exceptionally high by comparison with the highest attainable hardness in the ZK60 alloy of Hv = 105–110 after processing through five turns of HPT.39 Color-coded contour maps are available to provide visual displays of the variations in hardness within the cross sections of the HPT disks.40,41
Nanostructured Al and Cu Alloys with Enhanced Strength and Conductivity
Mechanical strength and electrical conductivity are the most important properties of conducting metallic materials used in electrical engineering. Today, there is a growing need in this field for innovative conductor materials with improved properties. However, high electrical conductivity and high strength are usually mutually exclusive as a result of the physical nature of these properties. Alloying of pure metals results in a significant increase of their mechanical strength, whereas the electrical conductivity drops because of the scattering of electrons at solutes and precipitates, provided the latter are densely spaced.44
Recent studies have shown that microstructural design in Al, Cu, and their alloys can result in a favorable combination of high mechanical strength with enhanced electrical conductivity.45,46 It was demonstrated that both properties are primarily controlled by the microstructure of these materials of which the grain size, morphology of second phases and their distribution, as well as the dislocation structure are the most important parameters. In this case, nanostructuring the alloys by SPD is of special interest, and this raises fundamental questions concerning new mechanisms of strength and electrical conductivity as well as the innovation potential for practical applications of nanostructured materials.47, 48, 49
Nanostructured pure copper would be an innovative solution for electric circuitry and connectors (e.g. in electrical engines and voltage current converters). In the field of microelectronics materials, and more precisely in copper interconnects, the electrical performance must not compromise the resistance to creep and electro-voiding when the channel and size of the system is reduced. In particular, mechanical properties become dependent on the sample size when the characteristic dimensions of the sample are below a few tens of micrometers. There are two reasons for this: (I) the microstructural scale (grain size) is sample size dependent and (II) the confinement of plasticity to small dimensions leads to new phenomena that make mechanical properties sample size dependent.46 The potential application of nanostructured Cu with improved wear resistance has been highlighted as a material for reversible electrical contacts46 where an optimal design for such contacts was also proposed.
An area where SPD technologies have come close to industry-scale applications is in the manufacturing of medical implants. In the quest for materials with high mechanical performance and good biocompatibility, titanium alloys have come to the fore as the materials of choice for permanent implants, including bone replacement and dental applications. In the case of titanium, significant efforts go into enhancing the strength characteristics of commercial-purity (CP) grades to avoid potential biotoxicity of alloying elements, especially in dental implants. In the case of magnesium alloys, a great challenge is the excessively high rate of their degradation, which is problematic in terms of both the durability of the implant and the high rate of hydrogen evolution during corrosion as in vascular stent applications.
Although grain refinement by SPD cannot resolve all of these issues, it has been extremely effective in enhancing the property profile of the candidate implant materials.56, 57, 58, 59, 60 Not surprisingly, the mechanical performance of CP Ti of biomedical grades was improved significantly upon processing by ECAP. A recent study of the properties of Ti processed by a combination of ECAP-Conform and drawing61 returned record values of the ultimate tensile strength (1330 MPa) and fatigue strength (620 MPa). What is less evident is that extreme grain refinement of the bulk of the metal down to the nanoscale appears to transpire to surface morphology, which turns out to be conducive for enhanced adhesion and growth of living cells. Indeed, proliferation of the preosteoblast cells,62 fibroblast cells,56 and stem cells63 on the polished surface of nanostructured Ti processed by ECAP was shown to be promoted by grain refinement. However, in the implant manufacturing industry, implants undergo special surface treatments, such as grit-blasting, plasma-spraying, acid-etching, and anodization.64 The effect of grain refinement of the bulk of the material on the surface characteristics, which in turn control fatigue properties and cellular response, may be weakened by such surface treatments. A recent study60 shed some light on the effect of sand-blasting combined with acid-etching (the SLA process65) on the fatigue performance of CP Ti. The study demonstrated that the SLA surface treatment of Ti with different bulk microstructures gave rise to different levels of surface roughness. A greater increment of fatigue strength was achieved for the CG variant of Ti. Nevertheless, the fatigue properties of CP titanium processed by ECAP followed by SLA treatment were superior to those of CG CP titanium.
It should also be understood that the exceptional improvement of mechanical properties of Ti by such SPD processes as ECAP or its modifications, while not causing a deterioration of cell response, are not necessarily accompanied with its appreciable enhancement. This has been demonstrated by in vivo assays based on histology and micro-CT analyses.66 Still, the overall performance of SPD-processed titanium makes it very suitable for bone and tooth replacement. The ultimate proof for that has been provided in a most recent clinical study.61
Among the Ti alloys, SPD-processed β-alloys of the Ti-Nb system have attracted special interest. Not only do they show good biocorrosion and biocompatibility properties, but they also have a favorable Young’s modulus close to that of bone. This helps to avoid the detrimental effects of stress shielding on the bone tissue healing.67 SPD processing ensures that the relatively low strength of as-cast Ti-Nb is significantly improved through grain refinement,68,69 suggesting that this material still qualifies for bone replacement applications. However, the SPD parameters need to be chosen carefully to avoid the occurrence of deformation-induced new phases that may raise the Young’s modulus of the alloy to undesirably high levels (see, for example, Panigrahi et al.68).
For temporary (bioresorbable) implants, magnesium alloys have advanced as favorite materials because of their high biodegradation rate. Current research focuses on improving the biocompatibility and the mechanical performance of these systems through variations in alloy composition, microstructure, and surface treatment. Mg-Zn-Ca alloys have proven to exhibit both these advantages at the same time.69 With respect to the time necessary for tissue healing, however, these alloys may degrade too quickly and the concomitant hydrogen evolution is faster than the human body can absorb. The degradation was found to take longer with less alloyed Mg systems,70 albeit at the cost of their strength. The application of SPD has shown to bring back or even surpass the original level of strength by means of grain refinement,70,71 phase formation, and the generation of vacancy agglomerates.72
In summary, the emergence of UFG materials for permanent and biodegradable medical implants demonstrates in an exemplary way the great potential that SPD techniques have in developing novel materials in general.
Thermoelectricity and Superconductivity
SPD processing activities concentrated on decreasing the denominator of Eq. 2 by a decrease of electrical resistivity ρ via reduced electron scattering or by a decrease of the thermal conductivity λ via enhancement of phonon scattering at a fixed absolute temperature T, leaving the other quantity unchanged or accepting only a slight increase in it; S denotes the so-called Seebeck coefficient. SPD processing has been undertaken with two groups of materials (for a detailed review, see Rogl et al.75): (I) Bi-Te alloys for low-temperature applications and (II) skutterudites for high-temperature applications.
The low-temperature thermoelectrics such as Bi-Te alloys exhibit a large crystal anisotropy that is more important for the resultant ZT value than the decrease of grain size leading to a smaller thermal conductivity through additional phonon scattering. HPT processing gave rise to an increased power factor S 2/ρ caused by a (110) texture contributing to both a low resistivity and a high Seebeck coefficient,76 whereas a real increase of ZT was achieved by the ECAP procedure77 by carefully choosing the ECAP temperature and path to obtain a high carrier mobility, thus minimizing the electrical resistivity and thereby achieving a figure of merit as high as ZT = 2.3.
The SPD impact on superconductivity was also studied for the Nb-47 wt.% Ti alloy, a well-known system used for superconducting magnets.87 T c decreased with increasing shear strain but rose again with annealing. Although the grain size of the material was comparable with the coherence length (about 8ξ),88 the trend of T c with the imposed strain was opposite to pure Nb89 as a result of the dissolution of Ti in Nb with increased HPT straining. The application of HPT in conjunction with subsequent annealing led to an increase in strength while T c was maintained above the value obtained after solution treatment.
SPD-Processed Hydrogen Storage Materials
SPD processing has been reported to lead to significant improvements in the kinetics of hydrogen storage in metallic materials, mainly those in Mg-based and Ti-based alloys.
SPD-Processed Nanocrystalline Semiconductors
The results of recent studies reported in this article demonstrate that various superior properties, both mechanical and functional, can be achieved in bulk nanostructured materials produced by SPD. These results shed light on the mechanisms underlying the special properties of these materials and open up avenues for their practical applications as new structural and functional materials. Recent discoveries have also demonstrated new opportunities for SPD processing with respect to improving the physical and chemical properties of materials. These include increased electrical conductivity, superconductivity, and thermoelectricity in metals and alloys; improved hydrogen storage capability; enhanced biocompatibility; and many other unique phenomena that are of interest for various functional applications.
As shown in this overview, over the last decade a solid scientific foundation has been laid for enhancing the properties of materials by SPD-induced nanostructuring through extensive research. A greater understanding has been gained of the defining role of the grain boundary structure and further nanostructural features, such as nanoclusters, nanoparticles, and nanotwins, on the deformation properties and diffusion transport mechanisms. These nanostructural features are closely related to the regimes of SPD in which they were produced as a result of extreme straining, high pressures, and/or unusual phase transformations. With this new knowledge, it is reasonable to anticipate that, in the not-so-distant future, nanostructural design by SPD processing will provide new breakthroughs in the development of various materials with superior properties for advanced structural and functional applications.
RZV is funded by the Russian Federal Ministry for Education and Science (Grant No. 14.B25.31.0017), YE is funded by the Australian Research Council (Linkage Grant LP100200072) and the Russian Federal Ministry for Education and Science (Grant No. 14.A12.31.0001), ZH is funded by a Grant-in-Aid for Scientific Research (S) from the MEXT, Japan (No. 26220909), TGL is funded by the National Science Foundation of the United States (Grant No. DMR-1160966) and the European Research Council (Grant Agreement No. 267464-SPDMETALS), MJZ is funded by the EU-Initial Training Network BIOTINET (Grant Agreement No. 264635) and the Austrian Research Promotion Agency (K-Project OPTIBIOMAT), and YTZ is funded by the U.S. Army Research Office (W911 NF-12-1-0009), the National Science Foundation of the United States (Grant No. DMR-1104667), and the China 1000 Plan program.
- 2.M.J. Zehetbauer and Y.T. Zhu, eds., Bulk Nanostructured Materials (Weinheim: Wiley, 2009).Google Scholar
- 6.S.H. Whang, ed., Nanostructured Metals and Alloys: Processing, Microstructure, Mechanical Properties and Applications (Cambridge: Woodhead, 2011).Google Scholar
- 12.R.Z. Valiev, A.P. Zhilyaev, and T.G. Langdon, Bulk Nanostructured Materials: Fundamentals and Applications (Hoboken: Wiley, 2014).Google Scholar
- 16.X.L. Wu, M.X. Yang, F.P. Yuan, G.L. Wu, Y.J. Wei, X.X. Huang, and Y.T. Zhu, PNAS (2016).Google Scholar
- 27.T. Mungole, P. Kumar, M. Kawasaki, and T.G. Langdon, J. Mater. Sci. 50, 3549 (2015).Google Scholar
- 40.B. Ahn, H.J. Lee, I.C. Choi, M. Kawasaki, J.I. Jang, and T.G. Langdon, Adv. Eng. Mater. (2016). doi: 10.1002/adem.201500520.
- 41.M. Kawasaki, B. Ahn, H.J. Lee, A.P. Zhilyaev, and T.G. Langdon, J. Mater. Res. 31, 88 (2016).Google Scholar
- 53.EN 50183, Overhead Power Line Conductors: Bare Conductors of Aluminium Alloy with Magnesium and Silicon Content (Bruxelles: European Committee for Standardization (CEN), 2002).Google Scholar
- 54.V.Kh. Mann, A.Y. Krokhin, I.A. Matveeva, G.I. Raab, M.Y. Murashkin, and R. Valiev, Light Met. Age 72, 26 (2014).Google Scholar
- 58.T.C. Lowe and R.Z. Valiev, Advanced Biomaterials and Biodevices, ed. A. Tiwari and A.N. Nordin (Wiley-Scrivener: Beverly, 2014), pp. 1–52.Google Scholar
- 62.Y. Estrin, C. Kasper, S. Diederichs, and R. Lapovok, J. Biomed. Nat. Res. A 90A, 1239 (2008).Google Scholar
- 66.Y. Estrin, H.E. Kim, R. Lapovok, H.P. Ng, and J.H. Jo, Biomed. Res. Int. 914764 (2013).Google Scholar
- 71.O. Kulyasova, R. Islamgaliev, Y.H. Zhao, and R. Valiev, 6th International Conference on Nanomaterials by Severe Plastic Deformation (NANOSPD6), ed. B. Beausir, N. Kasprzak, and L.S. Toth (Metz: University Press of Lorrain University, 2014).Google Scholar
- 72.J. Horky, A. Ghaffar, A. Grill, St. Pogatscher, B. Mingler, P.J. Uggowitzer, and M. Zehetbauer. Paper presented at the 6th international conference on nanomaterials by severe plastic deformation (NANOSPD6), Metz, 2014.Google Scholar
- 73.S.S. Nene, B.P. Kashyap, N. Prabhu, Y. Estrin, and T. Al-Samman, J. Mater. Sci. 50, 3041 (2015).Google Scholar
- 74.Y. Estrin, S.S. Nene, B.P. Kashyap, N. Prabhu, and T. Al-Samman, to be published (2016).Google Scholar
- 77.T. Hayashi, Y. Horio, and H. Takizawa, Metall. Mater. Trans. 51, 1914 (2010).Google Scholar
- 84.H. Suematsu, M. Kato, and T. Ishida, in 25th International Conference on Low Temperature Physics (LT25), PT 5a 150(5a) (2009), p. 052250.Google Scholar
- 86.S. Lee and Z. Horita, Metall. Mater. Trans. 53, 38 (2012).Google Scholar
- 88.C.P. Poole, H.A. Farach, R.J. Creswick, and R. Prozorov, Superconductivity, 2nd ed. (Amsterdam: Elsevier, 2007).Google Scholar